1 Chem. Rev. 1990, The Sol-Gel Process LARRY L. HENCH' and JON K. WEST Dq"nt of Materials Sc*mce and Enghwrhg, Advanced Materials Research Center, UnimrMy of Floryle. oakresville. Fknm Received May (Revised Manuscript Received October 27, 1989) Contents 1. Introduction 11. Sol-Gel Process Steps: An Overview 111. Hydrolysis and Polycondensation IV. Gelation V. Theoretical Studies VI. Aging VII. Drying VIII. Stabilization IX. Densification X. Physical Properties XI. Conclusions I. Infroducf/on Interest in the sol-gel processing of inorganic ceramic and glass materials began as early as the mid-1900s with Ebelmanl,* and Graham's3 studies on silica gels. These early investigators observed that the hydrolysis of tetraethyl orthosilicate (TEOS), Si(OC2H5),, under acidic conditions yielded Si02 in the form of a "glass-like material".l Fibers could be drawn from the viscous gel, and even monolithic optical lenses? or composites formed? However, extremely long drying times of 1 year or more were necessary to avoid the silica gels fracturing into a fine powder, and consequently there was little technological interest. For a period from the late through the gels became of considerable interest to chemists stimulated by the phenomenon of Liesegang Rings4& formed from gels. Many noted chemists, including OstwaldE and Lord Rayleigh,? investigated the problem of the periodic precipitation phenomena that lead to the formation of Liesegang rings and the growth of crystals from gels. A huge volume of descriptive literature resulted from these studiesg'o but a relatively sparse understanding of the physical-chemical principles? Roy and co-workersll-" recognized the potential for achieving very high levels of chemical homogeneity in colloidal gels and used the sol-gel method in the and 1960s to synthesize a large number of novel ceramic oxide compositions, involving AI, Si, Ti, Zr, etc., that could not be made using traditional ceramic powder methods. During the same period Iler's pioneering work in silica chemistry15 led to the commercial development of colloidal silica powders, Du Pont's colloidal Ludox spheres. Stober et a1.i6 extended Iler's findings to show that using ammonia as a catalyst for the TEOS hydrolysis reaction could control both the morphology and size of the powders, yielding the so-called Stober spherical silica powder. The final size of the spherical silica powder is a function of the initial concentration of water and ammonia, the type of silicon alkoxide (methyl, ethyl, c, Lany L. Hend, is a eadaduate Research Professa in tb Cep" 01 Materials Science and Engineering at the University of Florida. where he has taught since 1964 after receiving B.S. (1961) and Ph.D. (1964) degrees in Ceramic Engineering at The Ohm State Universny. He is the Director of lha Boglass Research Center and CoDirectof of the Advanced Materials Research Center at the University of Florida. He has published more than 250 research articles and is the coauthor or coeditor of 12 books in the fields of biomateriak. ceramic processing. ceramic characterization. glass surfaces. electronic ceramics. nuclear waste disposal, and sol-gel processing. r 4-7 Jon K. West received his Ph.D. at the Univerrity of FkMa in 1979 while wwking full lime as an engineering manager wilh tb Battery Business Department of General Electric Co. His cment position is Associate-in-Engineering with the Department of Materials Science and Engineering at the University of Florida. His work in sol-gel silica includes mechanical testing, process control and instrumentation. and theoretical studies based on molecular wbtal calculations. He is the author of eight publications Including the recently published textbook Principles of Electronic Ceramics. by Hench and West. from John Wilev 8 Sons. pentyl, esters, et4 and alcohol (methyl, ethyl, butyl, pentyl) mixture used,16 and reactant tempe~ature.~' An example of a typical colloidal silica powder is shown in Figure la, made by the Stober process, and its uniform distribution of particle sizes is shown in Figure lb from Khadikar and Sacks work.ls /90/ $09.50/ American Chemical Society
2 34 Chemical Reviews Vol. 90. No. 1 Hen& and West Tho,, MgO, TiO,, ZrSiO,, and 3AI2O3.2SiOzfibers.Abrasive grains based upon sol-gel-derived alumina are important commercial products." A variety of coatings and films have also been developed by using sol-gel methods. Of particular importance are the antireflection coatings of indium tin oxide (ITO) and related compositions applied to glass window panes to improve insulation c h a r a ~ t e r i s t i c s. ~ ~ Other work on sol-gel coatings is reviewed by Schroeder,'8 Macken~ie,'~," and Wenzel.S1 Mackenzie's rev i e ~ s ~ ~include 5 0 many other applications of the sol-gel process, proven, possible, and potential. The motivation for sol-gel processing is primarily the potentially higher purity and homogeneity and the lower processing temperatures associated with sol-gels compared with traditional glass melting or ceramic powder methods. Ma~kenzie'~fl summarizes a number of potential advantages and disadvantages and the relative economics of sol-gel methods in general. Hench and colleague^^^^" compare quantitatively the merits of sol-gel-derived silica optics over the alternative high-temperature processing methods. During the past decade there has been an enormous growth in the interest in the sol-gel process. This growth has been stimulated by several factors. On the basis of Kistler's early work,%several teams have produced very low density silica monoliths, called aerogels, by hypercritical point drying.5b Zarzycki, Prassas, and P h a l i p p o ~ demonstrated ~~.~ that hypercritical point.j.n...e.5.s.i drying of silica gels could yield large fully dense silica glass monoliths. Yoldassgshowed that large monolithic pieces of alumina could be made by sol-gel methods. Figure I. Top SEM of Stober spherical silica powders. Bottom: These demonstrations of potentially practical routes for Histogram (number of particles in a given diameter class versus particle diameter) of a typical batch of Stoher spherical silica production of new materials with unique properties powders. Reprinted from ref 18: copyright 1988 University of coincided with the growing recognition that powder Florida. processing of materials had inherent limitations in homogeneity due to difficulty in controlling agglomerao ~ e r b e e k ' ~and 3 SugimotoZ1showed that nucleation, tion.60 of particles in a very short time followed by growth The first of a series of International Conferences on without supersaturation will yield monodispersed colprocessing was held in 1983to establish loidal oxide particles. Matijevic and c o - ~ o r k e r s ~ ~ -Ultrastructure ~~ a scientific basis for the chemical-based processing of have employed these concepts to produce an enormous a new generation of advanced materials for structural, range of colloidal powders with controlled size and electrical, optical, and optoelectronic applications. morphologies, including oxides (TiO,, a-fepo3, Fe304, Support by the Directorate of Chemical and AtmosBaTiO,, Ce02), hydroxides (AIOOH, FeOOH, Cr(OH),), pheric Sciences of the Air Force Office of Scientific carbonates (Cd(OH)CO,), Ce,O(CO3),, Ce(III)/Y Research (AFOSR) for the Ultrastructure Conferences HC03), sulfides (CdS, ZnS), metals (Fe(III), Ni, Co), in 1983,6l 1985,6, 1987," and 198ga and the Materials and various mixed phases or composites (Ni, Co, Sr Research Society Better Ceramics Through Chemistry ferrites), sulfides (Zn, CdS), (Pb, CdS), and coated annual meetings in alternate years in 1984,6519S6,66and particles (Fe304with AKOH), or Cr(OH),). 198Sa has provided constant stimulation for the field. The controlled hydrolysis of alkoxides has also been used to produce submicrometer Ti0z,26doped Ti02.27 In addition, AFOSR has provided a stable financial base of support for a number of university programs in Zr0z,28 and doped Zr0z,28doped SiOz,TJSrTiO,." and sol-gel science throughout the 1980s under the technical even cordierite30 powders. monitoring of D. R. Ulrich. Emulsions have been employed to produce spherical The primary goal in these conferences and the powders of mixed cation oxides, such as yttrium aluafosr research and development program was to esminum garnets (YAG), and many other systems such tablish a scientific foundation for a new era in the as reviewed in Hardy et al." manufacture of advanced, high-technology ceramics, Sol-gel powder processes have also been applied to glasses, and composites. For millennia, ceramics have fissile elements31where spray-formed sols of U 0 2 and U02-PuO, were formed as rigid gel spheres during been made with basically the same technology. Powders, either natural or man-made, have been shaped passage through a column of heated liquid. into objects and subsequently densified at temperatures Both glass and polycrystalline ceramic fibers have close to their liquidus. The technology of making glass been prepared by using the sol-gel method. Compohas also remained fundamentally the same since presitions include TiOz-Si02 and Zr02-Si02 glass history. Particles are melted, homogenized, and shaped high-purity SiO, waveguide f i b e r ~? ~A120b. ~ ~ ZrO,,
3 The Sol-Gel Process Chemical Reviews, 1990, Vol. 90, No f Figure 2. Change in the roles of physics and chemistry as ceramics move toward ultrastructure processing. Reprinted from ref 61; copyright 1984 Wiley. into objects from the liquid. The goal of sol-gel processing and ultrastructure processing in general is to control the surfaces and interfaces of materials during the earliest stages of production.61 Long-term reliability of a material is usually limited by localized variations in the physical chemistry of the surface and interfaces within the material. The emphasis on ultrastructure processing is on limiting and controlling physical chemical variability by the production of uniquely homogeneous structures or producing extremely fine-scale ( nm) second phases. Creating controlled surface compositional gradients and achieving unique physical properties by combining inorganic and organic materials are also goals of ultrastructure processing. The concept ofmolecular manipulation of the processing of ceramics, glasses, and composites requires an application of chemical principles unprecedented in the history of ceramics. Modern ceramics are primarily the products of applied physics, as indicated in Figure 2. During the past decade there has been enormous progress made in the shifting of the emphasis of ceramic science to include a larger overlap with chemistry, as also illustrated in Figure 2.61 The extensive literature represented by the conference proceedings cited above6147 contains excellent examples of this shift toward chemical-based processing in materials science. Another essential factor for the increased scientific understanding of the sol-gel process is the availability of new analytical and calculational techniques capable of investigating on a nanometer scale the chemical processes of hydrolysis, polycondensation, syneresis, dehydration, and densification of materials. Many of the concepts of molecular control of sol-gel processes are a result of the use of nuclear magnetic resonance (NMR), X-ray small-angle scattering (XSAS), Raman spectroscopy, X-ray photoelectron spectroscopy (XPS), differential scanning calorimetry (DSC), dielectric relaxation spectroscopy (DRS), etc., that have been developed during the past three decades. The difference between the modern development of sol-gel-derived materials, such as gel-silica opti~s,~~-~~ and the classical work of Ebelman1*2 is that now drying of the monolithic silica optics can be achieved in days rather than years. The primary problem that had to be overcome was cracking during drying due to the large shrinkage that occurs when pore liquids are removed from the gels. For small cross sections, such as in powders, coatings, or fibers, drying stresses are small and can be accommodated by the material. For monolithic objects greater than about 1 cm in diameter, drying stresses developed in ambient atmospheres can introduce catastrophic fracture. To prevent fracture during drying, it is essential to control the chemistry of each step of the sol-gel process carefully. Likewise, to densify a dried gel monolith, it is essential to control the chemistry of the pore network prior to and during pore closure. The objective of this review is to describe the chemistry of the seven steps of the sol-gel process that can yield monoliths under ambient pressures. This review also describes how sol-gel-derived monoliths can be processed to result in fully dense components or with precisely controlled and chemically stable porosities. Most detail exists for Si02, and therefore the emphasis in this review is on silica sol-gel processing. The processing of silica monoliths by alkoxide methods will be compared with more traditional colloidal sol-gel methods. The reader interested in the sol-gel processing of compositional systems other than Si02 or coatings, fibers, powders, or aerogels is referred to the Conference Proceedings cited above6147 as well as an International Workshop on Sol-Gel and special conferences chaired by Sanders and Klein69 and Fri~ke.~~ Klein's volume on sol-gel techn~logy,~~ emphasizing thin films, fibers, hollow glass microspheres, and specialty shapes, illustrates many potential applications of this field. A textbook on sol-gel science has recently been completed by Brinker and S~herer.~~ Other general reviews on earlier work include those by Klein,71 Sakka and Kami~a,~~ M~kherjee,~~ Sakka,74i75 and of course Iler15976 and Okker~e.~~ II. Sol-Gel Process Steps: An Overview Three approaches are used to make sol-gel monoliths: method 1, gelation of a solution of colloidal powders; method 2, hydrolysis and polycondensation of alkoxide or nitrate precursors followed by hypercritical drying of gels; method 3, hydrolysis and polycondensation of alkoxide precursors followed by aging and drying under ambient atmospheres. Sols are dispersions of colloidal particles in a liquid. Colloids are solid particles with diameters of nm.78 A gel is a interconnected, rigid network with pores of submicrometer dimensions and polymeric chains whose average length is greater than a micrometer. The term "gel" embraces a diversity of combinations of substances that can be classified in four cate- gories as discussed by F10ry:~~ (1) well-ordered lamellar structures; (2) covalent polymeric networks, completely disordered; (3) polymer networks formed through physical aggregation, predominantly disordered; (4) particular disordered structures. A silica gel may be formed by network growth from an array of discrete colloidal particles (method 1) or by formation of an interconnected 3-D network by the simultaneous hydrolysis and polycondensation of an organometallic precursor (methods 2 and 3). When the pore liquid is removed as a gas phase from the interconnected solid gel network under hypercritical conditions (critical-point drying, method 2), the network
4 36 Chemical Reviews, 1990, Vol. 90, No. 1 Hench and West Figure 3. Gel-silica glass process sequence. powders made by chemical vapor deposition (CVD) of SiC The processing steps involved in making sol-gel-derived silica monoliths for methods 1-3 are compared below. A schematic illustration of these seven steps is given in Figure 3 for methods 1 and 3. Step 1: Mixing. In method 1 a suspension of colloidal powders, or sol, is formed by mechanical mixing of colloidal particles in water at a ph that prevents precipitation, as discussed in detail by Iler In methods 2 and 3 a liquid alkoxide precursor, such as Si(OR),, where R is CH3, CzH5, or C3H7, is hydrolyzed by mixing with water (eq 2). OCH, RELATIVE TIME I I does not collapse and a low density aerogel is produced. Aerogels can have pore volumes as large as 98% and densities as low as 80 kg/m3.59p80 When the pore liquid is removed at or near ambient pressure by thermal evaporation (called drying, used in methods 1 and 3) and shrinkage occurs, the monolith is termed a xerogel. If the pore liquid is primarily alcohol based, the monolith is often termed an alcogel. The generic term gel usually applies to either xerogels hydrolysis: H,CO-Si--OCH, + 4(H20) + ACH, OH H-Si-OH + 4(CH30H) AH TMOS + 4(H20) + Si(OH14 + 4(CHsOH) (2) The hydrated silica tetrahedra interact in a condensation reaction (eq 3), forming =Si-O-Si= bonds. OH I AH PH condensation: HO-Si-OH + HO-Si-OH + or alcogels, whereas aerogels are usually designated as HO-Si<-Si-OH + H,O (3) such. A gel is defined as dried when the physically AH AH adsorbed water is completely evacuated. This occurs between 100 and 180 "C. Linkage of additional =Si-OH tetrahedra occurs as The surface area of dried gels made by method 3 is a polycondensation reaction (eq 4) and eventually revery large P400 m2/g), and the average pore radius is sults in a Si02 network. The H20 and alcohol expelled very small (<IO nm). Larger pore radii can be Produced from the reaction remains in the pores of the network. by thermal treatment,220 by chemical washing during aging,237 or by additions of HF to the The small I I + pore radii can lead to large capillary pressures (eq 1) HO-Si-O-Si --OH + 6 W W 4 during drying or when the dried gel is exposed to liquids dh AH as described by Laplace's equation, discussed by Zar- HO zycki,81 and developed extensively by S ~herer~~,*~-~ for I I HO-Si-OH the drying of gels: I I HO Ap = 2y(cos 0)/r (1) o I I where Ap = the pressure difference in the capillaries, y = specific surface energy of the vapor-liquid interface, 0 = contact angle, and r = pore radius. HO-&-OH A dried gel still contains a very large concentration HA of chemisorbed hydroxyls on the surface of the pores. Thermal treatment in the range "C desorbs the hydroxyls and thereby decreases the contact angle and the sensitivity of the gel to rehydration stresses, resulting in a stabilized gel. Heat treatment of a gel at elevated temperatures substantially reduces the number of pores and their connectivity due to viscous-phase sintering. This is termed densification. The density of the monolith increases and the volume fraction of porosity decreases during sintering. The porous gel is transformed to a dense glass when all pores are eliminated. Densification is complete at "C for gels made by method 1 and as low as 1000 "C for gels made by method The densification temperature decreases as the pore radius decreases and surface area of the gels increases, as illustrated in Figure 3. Silica glass made by densification of porous silica gel is amorphous and nearly equivalent in structure and density to vitreous silica made by fusing quartz crystals or sintering of Si02 OH OH AH OH HO-Si-OH OH I 0 OH 1 I OH HO-Si-O-Si~-Si-O-Si<H + 6(H20) (4) HA d A AH HO-Li-OH The hydrolysis and polycondensation reactions initiate at numerous sites within the TMOS + H20 solution as mixing occurs. When sufficient interconnected Si-0-Si bonds are formed in a region, they respond cooperatively as colloidal (submicrometer) particles or a sol. The size of the sol particles and the cross-linking within the particles (i.e., density) depend upon the ph and R ratio (R = [H,O]/[Si(OR),]) among other variables discussed in a later section. Step 2: Casting. Since the sol is a low-viscosity liquid, it can be cast into a mold. The mold must be selected to avoid adhesion of the gel. Step 3: Gelation. With time the colloidal particles and condensed silica species link together to become a three-dimensional network. The physical characteristics of the gel network depend greatly upon the size of particles and extent of cross-linking prior to gelation. At gelation, the viscosity increases sharply, and a solid object results in the shape of the mold. With appro- AH I
5 The Sol-Gel Process Chemical Reviews, 1990, Vol. 90, NO priate control of the time-dependent change of viscosity of the sol, fibers can be pulled or spun as gelation occurs. Step 4: Aging. Aging of a gel, also called syneresis, involves maintaining the cast object for a period of time, hours to days, completely immersed in liquid. During aging, polycondensation continues along with localized solution and reprecipitation of the gel network, which increases the thickness of interparticle necks and decreases the porosity. The strength of the gel thereby increases with aging. An aged gel must develop sufficient strength to resist cracking during drying. Step 5: Drying. During drying the liquid is removed from the interconnected pore network. Large capillary stresses can develop during drying when the pores are small (e20 nm). These stresses will cause the gels to crack catastrophically unless the drying process is controlled by decreasing the liquid surface energy by addition of surfactants or elimination of very small pores (method l), by hypercritical evaporation, which avoids the solid-liquid interface (method 2), or by obtaining monodisperse pore sizes by controlling the rates of hydrolysis and condensation (method 3). After hypercritical drying (method 1) the aerogel has a very low density and is a very good thermal insulation when sandwiched between glass plates and eva~uated.5~ Step 6: Dehydration or Chemical Stabilization. The removal of surface silanol (Si-OH) bonds from the pore network results in a chemically stable ultraporous solid. Porous gel-silica made in this manner by method 3 is optically transparent with interconnected porosity and has sufficient strength to be used as unique optical components when impregnated with optically active polymers such as fluors, wavelength shifters, dyes, or nonlinear polymer~.~~t~~ Step 7: Densification. Heating the porous gel at high temperatures causes densification to occur. The pores are eliminated, and the density ultimately becomes equivalent to fused quartz or fused silica. The densification temperature depends considerably on the dimensions of the pore network, the connectivity of the pores, and surface area, as illustrated in Figure 3.89 Alkoxide gels (method 3) have been densified as low as 1000 "C by Klein and Garvey,2w whereas gels made by the commercial colloidal process developed by Shoupw require OC. However, colloidal silica gels with very carefully controlled dense packing can also be densified at low temperatures of 1000 "C, as shown by Sacks and T ~eng.~'~~~ The purity and homogeneity of dense gel-silica made by method 3 are superior to other silica glass processing methods. The ability to produce optics with nearly theoretical limits of optical transmission, lower coefficients of thermal expansion, and greater homogeneity, along with net shape casting, represents major advances resulting from sol-gel processing of monolith^.^^^^^ Details of these seven sol-gel processing steps follow. The emphasis is on sol-gel-derived silica monoliths made by the alkoxide process (method 3) processed under ambient pressures. I I I. Hydrolysis and Polycondensation As shown in Figure 3 the structure of a gel is established at the time of gelation. Subsequent processes such as aging, drying, stabilization, and densification all depend upon the gel structure. Since it is the relative rates of hydrolysis (eq 2) and condensation (eq 3) that determine the structure of the gel, it is essential to understand the kinetics of the hydrolysis and condensation reactions and the ratio of their rate constants (kh/kc) * As discussed by Orcel et a1.,93-95 Hench and Orce1,96 Klemperer et al,,w*98 Scherer and Brinker,70 and Artaki et al.,% many factors influence the kinetics of hydrolysis and condensation, and the systems are considerably more complex than represented by the simplified eqs 2-4. Many species are present in the solution, and furthermore, hydrolysis and polycondensation occur simultaneously. The variables of major importance are temperature, nature and concentration of electrolyte (acid, base), nature of the solvent, and type of alkoxide precursor. Pressure influences the gelation process also; kh increases with pressure as shown by Artaki et a1., but pressure is usually not a processing variable. There are relatively few studies of the dependence of kh and kc on independent processing variables. In fact many studies have reported the variation of the gelation time, viscosity, or textural characteristics (e.g., specific surface area) of the gel as a function of experimental conditions without determining kh or kc However, several investigations do provide a scientific foundation for understanding the processing dependence of kh and kc. Aelion's study of the influence of electrolyte concentration on the hydrolysis of TEOS in different solvents showed that kh increases linearly with the concentration of H+ or H30+ in acidic media and with the concentration of OH- in basic medium.lo3 The reaction rate varies from 4.12 X lo4 L mo1-ls-l for a mol L-l HC1 solution. This corresponds to a rate constant per unit concentration of electrolyte of mol L-l s-' [H+]-l. Similar values are observed in basic media where the rate constant is about L mol-' s-l [OH]-'. There is a variation in the concentration of TEOS of 0.2 mol L-l for the basic conditions versus 0.6 mol L-' for the acid-catalyzed sol. The increase in [TEOS] can account for the increase in rate constant. As discussed by OrceP the nature of the solvent (dioxane, methanol, or ethanol) has a "secondary" effect on kh, as well as the temperature dependence of the reaction (10-fold increase when the temperature varies from 20 to 45.5 "C). NMR experiments by Artaki, Zerda, and Jonas'OO show that kh varies in the different solvents as follows: acetonitrile > methanol > dimethylformamide > dioxane > formamide, with kh- (acetonitrile) being about 20 times larger than ItH(formamide). An increase of the R ratio (moles of water/moles of TEOS) from 1.86 to 3.72 induces kh to increase from to L mol-' s-l [acid]-l.lo3 However, Schmidt et al.lo4 found that the hydrolysis rate decreases when the R ratio increases from 0.5 to 2. Schmidt attributes this to the "special experimental conditions and the water acting as a proton acceptor which decreases the proton activity".lo5 The nature of the alkoxy groups on the silicon atom also influences the rate constant. As a general rule, the longer and the bulkier the alkoxide group, the slower the rate constant.105j08j09 For example, in the case of
6 38 Chemical Reviews, 1990, Vol. 90, No. 1 the hydrolysis of kh = 51 X L mol-l s-l [H+]-' for R = C2H5 and kh = 3 X 10" L mo1-ls-l [H+]-' for R = (CH3)2CH(CH2)3CH(CH3)CH2. From these results it is apparent that the dominant factor in controlling the hydrolysis rate is the electrolyte con~entration.~~ However, the nature of the acid plays an important role. As outlined above, a minute addition of HCl induced a 1500-fold increase of kh. However, Aleion reported "hydrolysis in glacial acetic acid as solvent is not particularly fast".lo3 Although these have been called "secondary" effectslo3 and they are very small compared to those induced by addition of electrolyte, they are relatively important (e.g., the 10-fold increase of kh with a variation of the processing temperature of 25.5 "C) and might be responsible for numerous observations in systems investigated in other works. For example, a systematic study of Mackenzie shows that the type of acid catalyst and nature of solvent have a large effect on TEOS gelation.l1 Although the polycondensation of silicic acids has been studied extensively, as reviewed by Iler15376 there are little data on the rate constant of the condensation reaction.93 A value of kc = 3.3 X lo+ L molw1 s-l has been reported by Artaki et al. for the dimerization of monosilicic acid.lo2 However, no value of kh is available for the same system. Artaki et al. showed that application of a pressure of 5 kbar to the system increased the polycondensation rate constant by a factor 10.'O2 There are many problems associated with the computation of reaction rate constants and especially the determination of the mechanisms of the reactions as well as the order of the reactions with respect to the constituents, as discussed by Schmidt et al.lo5 When the order of the reaction varies with time, such as in Uhlmann et al.'s experiments, determining the rate constant becomes even more difficult.lw For short periods of time, the order of the reaction can be considered constant. However, one must keep in mind that there are several hydrolysis and condensation reactions possible, each having its own rate c~nstant.~~~j'' Consequently, assumptions are necessary to allow the computation of kh and kc, which limits the characterization of the reactions to the early stages of the process. Because of the above limitations, early studies of the influence of the experimental factors on the sol-gel process were primarily phenomenological, without specific values of the ratio kh/kc being determined for a single system. This situation has changed dramatically in the past few years. Many investigators have pursued the kinetics of silicon alkoxide hydrolysis using 29Si NMR. It is one of the most useful techniques to follow the hydrolysis and first-stage polymerization of silicon alkoxide, because it allows the determination of the concentration of the different Si(Or),(OH), and (OH),(OR),Si-0-Si(OR)x(OH), species. Each of the monomer and dimer species has a specific chemical shift with respect to the metal alkoxide.'12 Engelhardt et employed 29Si NMR as early as 1977 to investigate the condensation of aqueous silicates at high ph. Their results indicate that a typical sequence of condensation products is monomer, dimer, linear trimer, cyclic trimer, cyclic tetramer, and a higher order generation of discrete colloidal particles which are commonly observed in aqueous systems. This sequence Hench and West Figure 4. Variation of the concentration of M1 (Si(OH)(OCH,),) and D1 ((OCH3),Si-O-Si(0CH3),) as a function of time for the different solution^.^^ of condensation requires both depolymerization (ring opening) and availability of monomers (species that may be produced by depolymerization). However, in alcoholic solutions especially at low ph the depolymerization rate is very low. Iler15 speculates that under conditions where depolymerization is least likely to occur, so that the condensation is irreversible and siloxane bonds cannot be hydrolyzed once they are formed, the condensation process may resemble classical polycondensation of polyfunctional organic monomers resulting in a three-dimensional molecular network. Owing to the insolubility of silica under these conditions, the condensation polymer of a siloxane chain cannot undergo rearrangement into particles. In sol-gel systems commonly employed for glass preparation, the water/alcohol ratio and ph are widely varied. Thus the importance of the reverse reactions depends on processing conditions, and it is anticipated that condensation may result in a spectrum of structures ranging from molecular networks to colloidal particles. Yoldas114 concluded that the hydrolysis reaction and the condensation reaction are not separated in time but take place simultaneously. It has been well established that the presence of H30+ in the solution increases the rate of the hydrolysis reaction, whereas OH- ions increase the condensation reaction.'15 Orcel et al.9* explored the effect of acid catalysis and formamide (a drying control chemical additive) on the hydrolysis and polycondensation rates of a TMOS silica system, using 29Si NMR. By plotting the variation of the concentration of the species of interest from the NMR data as a function of time (Figure 4), one can obtain the rate constants for hydrolysis (kh) and polycondensation (k,) of the Si alkoxide, in this case TMOS. Even though the assumptions involved in the computation of the rate constants are crude, such as firstorder kinetics and no influence of the degree of substitution of Si atoms on the reaction rates, the order of magnitude of kh and kc, Table I, demonstrates im-
7 The Sol-Gel Process TABLE I. Physicochemical Characteristics of the Different Gel Solutions sample SW 55 SF 25 SF 50 SF 23 vol formamide/vol formamide MeOH H20 103kH, L mol" h-i D1 D1 D1 ph=3 12 I 2 25 kc, L mol-' h'' d, nm portant differences. These data show that acid catalysis increases the hydrolysis rate constant, kh, by a factor of 2. The data also show that formamide decreases the hydrolysis rate and slightly increases the condensation rate. This can be attributed to the ability of HCONH2 to form hydrogen bonds and to its high dielectric constant (E = 110).ll6 The presence of formamide also decreases the time of gelation (tg). Additional details regarding the use of formamide and other drying control chemical agents (DCCAs) are discussed in refs 93 and 117. The studies of Klemperer and colleagues97~98 provide some of the most detailed evaluation of the extent of hydrolysis and condensation of silica prior to the onset of gelation. To identify the polysilicate intermediates formed during sol-gel processing, Klemperer et al.97 used a protocol that combined quenching by diazomethane, fractionation using spinning band column distillation, identification by capillary gas chromatography, and structural characterization using 29Si(1Hj NMR techniques (one-pulse, 1D-INADEQUATE, and 2D- INADEQUATE) to provide structural assignments and response factors for the components separated by gas chromatography. Theyg8 showed that under acidic conditions the polysilicate molecular size distributions, expressed in terms of mole percent of total silicon present as a function of degree of polymerization, exhibit maxima near the number-average degree of polymerization. There are mostly linear structures under acidic conditions. In contrast, under basic conditions the maximum of the distribution is at the monomer percent and extends to very high molecular weights. Thus, the distribution of polysilicate species is very much broader for basic conditions of hydrolysis and condensation, characteristic of branched polymers with a high degree of cross-linking, whereas for acidic conditions Klemperer et algs conclude that there is a low degree of cross-linking due to steric crowding. Raman spectroscopy is one means of assessing qualitatively the size of particles or scale of structure1l8jl9 when gelation occurs. Since the Raman intensity is proportional to the concentration of scatterers, sols and gels prepared with different experimental conditions can be compared by using a proper internal standard. In the study of the Si02-formamide system, methanol was used for calibration.9h5 According to the NMR data, the concentration of CH30H is constant after 0.7t at 23 "C, and the solvent is significantly expelled hom the gel after -6tg. Thus the calibrated Raman intensities are valid in the time frame 0.7tg-6t,. Results for several gel solutions, with and without formamide, under basic and acidic conditions, are given in Figure Lg6 These curves demonstrate that when formamide is present, i.e., samples SF 50 and SF 25, larger particles are formed at the gelation point. This is in good agreement with the NMR result^.^^-^^ Since formamide decreases the hydrolysis rate, fewer sites are a I / f d Chemical Reviews, 1990, Vol. 90, No I -,, 1 Reduced time (t/tql Figure 5. Variation with time of the relative Raman intensity of the 830-cm-' band of the various gel solutions.% available for condensation and larger particles are formed in the so1.93j17 The reaction of silica colloids with molybdic acid, a technique widely used for the characterization of soluble silicates,120 can also be used to assess the size of particles developed in the sol. Si02 particles depolymerize in an acidic medium, and the monosilicic acid thus formed gives a yellow complex with Mo, which can be measured optically. A plot of the absorbance as a function of time allows the computation of the depolymerization rate constant, kd, as a function of time.93p96 For example, the values of kd at 0.5tg for several SO2-formamide solutions can be used to calculate the particle diameter. Ultimately, kd can be related to the particle diameter d through an empirical law: log d = a + b log kd (5) where a and b are constants (see Iler120) depending on experimental conditions, mainly solution ph. Since the solution ph of samples 55, 25, and 50 are nearly equivalent, it is possible to compare relative particle sizes by using eq 5 and assuming the values for a and b from Iler.120 (Note: This is only an approximation since Iler's values are based on a ph = 2, SiOp solution.) The calculated values at the gelation point, shown in Table I, increase with increasing formamide concentration. It has been shown93194 that the calibrated Raman intensity IR is inversely proportional to kd Thus, IR can be related to the sol particle size as IR = Adlfb (6) where A is a function independent of d. For the conditions described by Iler" l/b = The theoretical basis for this value is developed in refs 93 and 94. By use of l/b and the values of d (eq 5) calculated from the Mo test, it is possible to compute an empirical value of 6.8 for A in eq 6. By use of eq 6 and the measured values of Raman intensity (Figure 5), the time-dependent change in sol particle size can be calculated. The results are shown in Figure 5 on the right-hand particle-size axis. By the time of gelation, the size of the sol particles grows to 2 nm without formamide, and with 50% formamide they grow to 2.5 nm. These findings are similar to those of Klemperer et a in their studies of the effects of base vs acid d
8 40 Chemical Reviews, 1990, Vol. 90, No. 1 Hench and West TABLE 11. Chemical Characteristics of the TMOS Solutions (from Ref 94) lot3 kh, vol fract CH30H gelation soln mol h mol h in solv, 90 time, h I 2 > I n20moa MOLL RATIO: 20 HN0,fTEOS MOLL RATIO: 0.01 catalysis on the size of polysilicate species prior to the onset of gelation. Thus, Orcel et al. s studiesg4 show that the shape and size of polymeric structural units are determined by the relative values of the rate constants for hydrolysis and polycondensation reactions (kh and kc, respectively). Fast hydrolysis and slow condensation favor formation of linear polymers; on the other hand, slow hydrolysis and fast condensation result in larger, bulkier, and more ramified polymers.lm As illustrated by the values of kh and kc reported in Table 11, larger particles are anticipated for solution 1 (higher volume fraction CH30H in the solvent), which implies a lower value for the depolymerization rate constant: ki < hii. By combination of these various analytical methods, the particle diameter (PD) of the silica particles in the sol at the different steps of the sol-gel process can be estimated. The re~ults~j~~ are given in Table 111, and it is possible to conclude that the particles are about 20 A in diameter at the gelation point and larger particles are formed when formamide is present in the solution, as discussed in the next section on gelation. IV. Gelaflon The gelation point of any system, including sol-gel silica, is easy to observe qualitatively and easy to define in abstract terms but extremely difficult to measure analytically. As the sol particles grow and collide, condensation occurs and macroparticles form. The sol becomes a gel when it can support a stress elastically. This is typically defined as the gelation point or gelation time, tgel. There is not an activation energy that can be measured, nor can one precisely define the point where the sol changes from a viscous fluid to an elastic gel. The change is gradual as more and more particles become interconnected. All subsequent stages of processing depend on the initial structure of the wet gel formed in the reaction bath during gelation. Brinker and SchererlZ1 point out that the sharp increase in viscosity that accompanies gelation essentially freezes in a particular polymer structure at the gel point. At this point gelation may be considered a rapid solidification process. This frozen-in structure may change appreciably with time, depending on the temperature, solvent, and ph conditions or upon removal of solvent. A. Gelation Time A number of investigators have shown that the time of gelation changes significantly with the sol-gel chem- 0.1 t 0 SO SO TIME lhrl Figure 6. Loss tangent as a measure of gelation time (Sacks and Sheu, 1986). (A) Plots of storage modulus and loss modulus vs aging time for sol 1. (B) Plot of loss tangent vs aging time for sol 1. istry.15~95~117~122~1z3 One of the most precise methods to measure tgel was developed by Sacks and Sheu.lZ4 This method measures the viscoelastic response of the gel as a function of shear rate. They measured the complex shear modulus, G, by using a viscometer with a narrow gap. This ensures a well-defined shear rate as the cylinder in the sol oscillates at a frequency w and a small amplitude y. The complex shear modulus has the form G = G (w) + ig (w) (7) where G = storage modulus and G = loss modulus. The storage modulus arises from the elastic component of the sol-gel, while the loss modulus comes from the viscous component. The relative measure of the viscous energy losses to the energy stored in the system is usually defined as the loss tangent: tan 6 = G /G (8) Figure 6 shows the large change in the loss tangent at the gelation time along with the changes in Gr and G from Sacks and Sheu.lZ4 The rapid increase in the storage modulus near tgel is consistent with the concept that the interconnection of the particles becomes suf- I TABLE 111. Structural and Textural Properties of the Gels (from Orcel et a1.ls6)n property PD, A PR, A PV, cm3/g SA, m2/g.- D1, 8, D2, 8, 4 soln I (with DCCA) soln I1 (no DCCA) PD, particle diameter (Mo test); PR, pore radius; PV, pore volume; SA, specific surface area; D1, Guinier radius at gelation point; D2, Guinier radius on film heated at 200 C; df, fractal dimension at gelation point.
9 The Sol-Gel Process Chemical Reviews, 1990, Vol. 90, No GELATION TIME I R Figure 7. Variation of the gelation time with the R ratio.'% ficient to support a load elastically. There is at least one indication that gelation time (t,) is not an intrinsic property of the sol: t, depends on the size of the container. Furthermore, gelation may occur at different extents of reaction completion. For example, in the case of the polymerization of TMOS, more silicon alkoxide must be hydrolyzed when the experimental conditions favor a ramified polymer rather than a linear one. The dependence of t, on solution ph has not been fully determined, but it appears from the work of Yamane et al. that the curve t vs ph has a bell shape.'25 In other words, gelation can be nearly instantaneous for very acidic or basic solutions of metal alkoxides. This behavior is very different from the gels prepared by destabilization of a silica sol where the curve has a S shape with the maximum around the isoelectric point of silica (ph - 2) and a minimum near ph However, it should be noted that two solutions with the same ph may have different gelation times, depending on the nature of the counterion, all other parameters being equal. The anion and solvent also play a role in the kinetics of gelation,"o and gelation can be either acid or base c ataly~ed.~~j~~j~~ It is difficult to separate the effect of the alkoxy group from the effect of the solvent since gelation kinetics depends on the quantity of the solvent concentration. However, the trend is the longer and the larger the solvent molecule, the longer the gelation time. Similarly, Mackenzie has shown that the longer and the larger is the alkoxy group, the longer is t,.ll0 The amount of water for hydrolysis has a dramatic influence on gelation time (Figure 7) from Colby et al.'% For a R ratio (moles of water/moles of silicon alkoxide) of 2, t, is about 7 h (gelation process at 70 "C with HF as catalyst) and decreases to 10 min for R = For low water contents, generally an increase of the amount of hydrolysis water decreases the gelation time, although there is a dilution effect. It can be predictedg3 that for higher water contents, the gelation time increases with the quantity of water. The location of the minimum in the curve t, vs R, such as shown in Figure 7, depends on the experimental conditions, such as nature of the chemicals, catalyst, and temperature. Polymerization reactions are usually thermally activated, and this is observed for the hydrolysis and polycondensation of solutions of silicon alkoxides. For example, Mackenzie has shown that a molar solution of TEOS in methanol gels in 49 h at 4 "C, in the presence of HF, and in about 0.3 h at 70 OC.llo Although it is important to know how t, varies with various experimental parameters, the knowledge thus developed is empirical and qualitative, and a better description of the system is needed in order to optimize the process. B. Viscosity of the Sol-Gel System The sol-gel process has the unique advantage of allowing the preparation of the same composition, such as silica, in markedly different physical forms, fibers, coatings, monoliths, just by varying a few experimental conditions. As reviewed by Or~el,~~ the processing parameter that must be controlled is the viscosity of the sol-gel system. For example, the casting density of a sol was shown by Klein and Garvey to be the determinant in the manufacture of monoliths (between 1 and 1.2 g/cm3 for acid-catalyzed TEOS).'29 Several investigators have shown that fibers can be drawn from a sol only for a range of viscosity that is greater than 1 Pa s.73,75j3e133 Coatings can be applied with the most efficiency when the concentration of oxides is within certain limits (several tens of grams of oxide per liter) which fix the visco~ity.~~j~~-~~~ Controlling these processes requires understanding the rheological properties of the sol-gel system. However, there are few quantitative studies relating gelation to rheological variables.'% Some attempts have been used to define the point of gelation by associating gel formation with a sudden increase of the viscosity or reaching a maximum of viscosity.l30,132,'40,141 The viscosity of a solution undergoing hydrolysis and polycondensation is time dependent and is related to the size of the particles. The larger the molecules, the higher the viscosity. Thus, any variation of the processing parameters that induces an increase of the apparent size of the particles increases the viscosity. For example, acid-catalyzed silica sol-gel samples have a higher viscosity than neutral or base-catalyzed solu- tions. 130,142 The effect of the concentration of water on viscosity is more complex. OrceP reviews the general behavior as follows: at low water content, an increase of the amount of H20 increases viscosity, which reaches a maximum and then decreases for a further increase of the concentration of water.'42 A similar effect is obtained by varying the concentration of silicon alkoxide.143,144 Sacks and Sheu's rheological studies124 show that a silica sol prepared with the alkoxide process goes from a Newtonian behavior to shear thinning and, finally, thixotropy, which is especially useful in describing the sol-gel transition. Furthermore, they dem~nstrated'~~ that spinnability is possible only when the solution is shear thinning or slightly thixotropic. C. Sol Structure The rheological data summarized in the preceding section demonstrate that there is a major evolution of structure during the sol-gel transition. The system evolves from a sol, where there are individual particles more or less weakly interacting with each other, to a gel, which basically becomes a continuous molecule occupying the entire volume. Consequently, it is important to characterize the evolution of the structure of the sol
10 42 Chemical Reviews, 1990, Vol. 90, No. 1 Hench and West I.75 I sw I I 1 I t 1 I I Loo h Figure 8. Variation with time of log I(h) vs log h curves for a SW55 sample (no f~rmamide).'~~ during the gelation process. Only a few techniques are available to follow structural evolution at the nanometer scale of sol-gels. They include small-angle X-ray scattering (SAXS), neutron scattering, and light scattering, each of them giving complementary information, and transmission electron microscopy. Small-angle X-ray scattering allows the determination of a characteristic length of the particle (Guinier's radius of gyration, or electronic radius of gyration) and a fractal dimension, which gives some information on the structure of the polymer (branched vs linear) and on the growth mechani~m.'~~ The application of SAXS to a number of gel systems has been reported by various a ~ t h o r s. ~ ~ ~ ~ ~ ~ ~ ~ ~ - ~ ~ ~ Small-angle neutron scattering (SANS) has also been applied to the study of silica ~ 0ls.l~~ Results similar to those from SAXS are obtained, but further developments of the SANS technique may produce additional insight to the sol-gel process.158 Light scattering has been used for a long time to characterize macromolecular solutions. Although this technique should be useful in following the sol-gel transition, it has received very little attention in the sol-gel literature. However, the characteristic dimension probed by visible light scattering is >10 nm, and therefore it cannot be used to characterize the early stages of the gelation process.149 Recent development of short-wavelength UV lasers may make it possible to extend light-scattering studies to the range of 3 nm and thereby could follow most of the gelation process. The major conclusion of the various scattering studies is that acid-catalyzed sols develop a linear structure with very little branching. In contrast, base-catalyzed systems are characterized by highly ramified structures. 150,?51 Figure 8 is a Porod plot showing SAXS scattering curves typical of a sol prepared by hydrolyzing TMOS.93J56 The log of the scattering intensity, I, is plotted as a function of the scattering factor h. The scattering factor is defined as h = (4r/X) sin (8/2). As time increases from the sol stage (t/t, = 0.11) toward gelation (t/t, = 1.00), there is an increase in the size of X-ray scatterers. However, after a critical time (t/t, Figure 9. 2 = 3; N = total number of bond sites = 43; n = total number of node bonds = 81: P = 0.7. = 0.28) no new scattering centers are formed. When formamide is present, the critical reduced time for formation of scattering centers is longer.93 The fractal nature of the network formed can be calculated from the slope of the Porod plot and is discussed in a later section, as are additional SAXS investigations. D. Classical or Mean-Field Theory of Gelation The classical or mean-field theory of polymerization was developed by F10ry.~~ The basis structure of this model looks like a tree and is called a Cayley tree or Bethe lattice. Figure 9 shows a Cayley tree model for a polymer that forms a connected, gel-forming cluster without forming rings. In this tree, the functionality or maximum number of bonds, z, that are allowed to form at each numbered bond site is 2=3 Other polymers have different values for this parameter. For example, silicic acid has a functionality of z = 4. Four bonds may form at every site where silicon is present. Returning to our model with z = 3, we can define the probability, P, of a bond forming at each site: p= number of bonds total number of node bonds (9) P = n/(nz) (10) where n = number of node bonds, N = number of sites, and z = dimensionality of the polymer. Thus, in our simple example, shown in Figure 9 N = 43; z = 3; n = 81 (11) This means that some bonds are counted twice. The number of connections for each numbered node is counted. For example (a) node 34 has one bond, (b) node 27 has two bonds, and (c) node 1 has three bonds. Therefore, the probability for a connection for each site in this example is P = n/(nz); P = 81/[(43)(3)]; P = 0.6 (12) This example forms a gel, as we have conceptually defined it, since the cluster is continuously connected from one side to the other. Thus, there must be at least two connections per node for the cluster to be a gel. This defines the critical probability, P,, for gel formation to be P, = 1/2 (13) or in terms of the functionality of the polymer324 P, = l/(z - 1) (14)
11 The Sol-Gel Process Chemical Reviews, 1990, Vol. 90, No a b Figure 10. Site percolation model: (a) empty grid; (b) Raman filling of grid. This defines then the degree of reaction at the gel point. The distribution of molecular weights can also be determined. However, there is a fatal flaw in this model. Because no rings are allowed, there is an increasing number of nodes as the radius of the cluster increases. In fact, the mass of this type of cluster increases as the fourth power of the radius as shown by Zimm and St~ckmayer'~~ and de Gennes." In real materials the mass must increase linearly with volume as the third power of the radius. However, this model is still useful in visualizing the gelation of silica sol-gels. It yields a degree of reaction of one-third: P, = l/(~ - 1) = 1/3 (15) at the time of gelation. That means that two-thirds of the connections are still available and play a role in subsequent processing. This value is lower than the experimental evidence as we shall see in the next section. It does however represent the minimum degree of reaction before gelation can occur as presented by F10ry.~~~ E. Percolation Theory Percolation theory and its relationship to gelation has been reviewed by ZallenlG1 and Stauffer et Percolation allows for rings or closed loops to form, and thus the mass of percolation models increases with the cube of the radius. Figure 10 shows a simple percolation model. Starting with an empty grid (Figure loa), intersections are randomly filled with particles (filled circles). If two circles or particles are adjacent, then bonding will occur (Figure lob). Loops of various sizes may form as the Figure 11. Bond percolation model. structure expands. This eliminates the fatal error of the classical model and is called a site percolation model. In a manner similar to the classical model, the probability, P, that a site may be filled is defined as P = n/n (16) where n = number of filled sites and N = total number of sites. With the simple example in Figure 10 Thus n = 32 (17) N = 64 (18) P = 1/2 (19) This simple model shows that for this value of site filling, complete connectivity or gelation is unlikely for the site model. Experimental results indicate that 0.6 C P, I 0.84 (20) for silica sol-gel systems, as reviewed by Zarzycki.81 Thus, this model must be modified to increase the connectivity. By starting with all the sites filled and randomly adding bonds, the connectivity increases over the site model. Figure 11 shows a bond percolation model. Again we can define the probability of bonding as P = n/n (21) where n = number of bonds and N = total number of bond sites. In the case of the example in Figure 11 we have n = 39 (22) N = 112 (23) P = 0.35 (24) where gelation appears likely. The bond percolation model is dependent on the lattice. Table IV shows a summary of the percolation threshold for various lattices based on Brinker and Scherer.'O The table also shows the volume fraction, &, of the gel at gelation and the filling factor, u. F. Fractal Theory The fractal model of structures was designated as such by Mandelbr~tl~~ gives order to the many seemingly random patterns generated by nature, such
12 44 Chemical Reviews, 1990, Vol. 90, No. 1 Hench and West TABLE IV. Percolation Threshold for Various Lattices (from Brinker and Scherer'O) dimensionality d latticea coordination z 1/(z - 1) Pc bond pesite filling factor = up,bib I chain triangular square kagom honeycomb fcc :i bcc SC diamond :i repb sc fcc SC fcc SC fcc = face-centered cubic; bcc = body-centered cubic; sc = simple cubic; rep = random closed-packed. bless precise values, determined experimentally. t CL U x.- ul c a n \ Fraitai C. 0. 't Size, R - Figure 12. Density of fractal objects. as trees,163 galaxies,164 or the surface of the sun.165 Witten and Sar~derl~J~~ and Witten and Cates168 have demonstrated the fractal nature of diffusion-limited aggregation of particles. Growth processes that are apparently disordered also form fractal objects.168 Sol-gel particle growth has also been modeled by using fractal concept~.~~j~~j~~ The nature of fractals requires that they be invariant with scale. This is a symmetry that requires the fractal to look similar no matter what level of detail is chosen. For example, a tree as a whole has a very similar structure as a small branch within that tree. The second requirement for mass fractals is that their density decreases with size (see Figure 12). Thus, the fractal model overcomes the problem of increasing density of the classical model yet retains many of its desirable features. Fractal objects are quantified by their fractal dimension, df. Figure 13 shows objects with increasing fractal dimension.70 For linear-like structures 1<d,<2 (25) (as shown in Figure 13B). Fractally rough structures have a mass fractal dimension 2<d,<3 (26) Figure 13. Fractal objects: (A) linear structures, 1 < df < 1.5; (B) fernlike structures, 1.5 < df < 2; (C) fractally rough structures, 2 < df < 3; (D) solid structure, df = 3. Reprinted from ref 70; copyright 1989 Academic Press. TABLE V Keefer's hydrolyzed monomer fractal dimension df nonfractal 100% triple 3 fractal 33% double % triple 33% fully fractal 50% double % fully (as shown in Figure 13C). Finally, uniform nonfractal objects have a fractal dimension df = 3 (27) (as shown in Figure 13D). The mass of a fractal then is related to the fractal dimension and its size or radius, R, by M a Rdi (28) Therefore, computer models can be constructed to generate particle growth and measure the resulting fractal dimension. One such fractal gelation model was developed by Keefer.153 He postulated that sol particles grow from partially hydrolyzed TEOS (Si(OC,H,),). When fully hydrolyzed TEOS was used in the model, a fully dense particle was formed that had no fractal nature.
13 The Sol-Gel Process Chemical Reviews, 1990, Vol. 90, No "I, 2 a /,,,,,,,, h(pl 1 Figure 14. Small angle X-ray scattering curves (slit smeared) from 1 M solutions of Si(OC,H,), hydrolyzed with varying amounts of H,O; 0.01 NHIOH was used as a catalyst. Reprinted from ref 153; copyright 1986 John Wiley & Sons, Inc. Table V shows selected models with varying degrees of hydrolysis. This model yields values for df similar to those found experimentally through SAXS. G. Small-Angle X-ray Scattering (SAXS) Fractal particles with a radius of approximately 20 nm may be studied by SAXS. It can be shown (see ref 93 for a detailed review of this theory), that the scattered intensity (0 of X-rays for small angles is related to the fractal dimension of the particle, df: I(h) a h-df (29) h = 4?r(sin a)/y (30) where 2a = scattering angle and X = wavelength. Additionally the monomer involved in the fractal particle must be small: R, >> h-' >> a (31) where R, = radius of gyration and a = primary particle radius. The radius of gyration is basically the radius of the scattering center derived from the number of scattering centers, N, per unit volume, u. This leads to the equation for the scattering intensity known as Guinier's 1aw: J69 I(h) = Npe2u2 exp[-'/rp2h2] (32) where pe = electronic density. Figure 14 shows SAXS curves for various TEOS and HzO sols with different R ratios, from Keefer's studie~.'~~ As the water content increases, (increasing R), the fractal dimension increases. That is, the particles become more dense. The primary particle of radius, a, is between 1 and 2 nm as shown by Orcel et al.94 and can be modeled by rings and chains of three to four silica tetrahedra. The secondary fractal particle has a radius, R,, of 5-20 nm as seen from SAXS.lZ2 For the TMOS-based sols investigated by SAXS, Figure 8 shown earlier, the fractal dimension, df, in- lo REDUCED TIME ( t/tg) Figure 15. Time evolution of electronic radius of gyration (Eo) and fractal dimension (D) of a SW55 s01ution.l~~ ---f nm m Figure 16. Schematic representation of primary and secondary particles in a TMOS-based alkoxide gel. creases with time as does the Guinier radius (RJ. This behavior is shown in Figure 15 based on the data of Figure 8. The structure reaches a fractal dimension around 2.3 at the gelation point. Table V summarizes results of the structural and textural properties for two TMOS + HzO solutions, with and without formamide as a DCCA.156 Near the gelation point the sols prepared from TMOS and HzO are formed of particles of about 6.0-nm diameter compared to scattering units of about 2.0-nm diameter for the films.156 Dilution experiments showed that the radius of gyration measured in the sols does not vary with the quantity of s~lvent.~~j~ This result indicates first that the Guinier approximation is valid for these systems and second that the polymer is relatively rigid.152 These measurements are in very good agreement with the values obtained by the Mo acidic test.93 These results suggest that the gel structure is formed of different units, e.g., primary particles of about 2.0-nm diameter that agglomerate in secondary particles of about 6.0-nm diameter (Figure 16). On the basis of geometric considerations, these secondary particles contain at most 13 primary particles. Gelation occurs when the secondary particles are linked to each other, forming a three-dimensional network across the sample. Aggregation of particles carrying a surface charge can be modeled by the classical Derjaguin-Landau-Verwey-Overbeek (DLVO) theory."' This theory predicts
14 46 Chemical Reviews, 1990, Vol. 90, No. 1 that the activation barrier to aggregation increases linearly with the size of two equal particles. Thus, the rate of aggregation would decrease exponentially with their size. Smaller particles however will aggregate with larger ones at a much higher rate. Thus, two distributions of particles are predicted, small newly formed particles and large aggregating particles.325 This description of the structure of the sol and gel is confirmed by another X-ray diffraction study by Himmel et al.170 They showed that gels manufactured from hydrolysis and polycondensation of TEOS by a small amount of acidic water are made of primary particles of about 1.0-nm diameter that associate in secondary chainlike clusters. The size of these clusters can be approximated as 6.0 nm in diameter, which is the average diameter of the pores. Also, TEM experiments on silica particles prepared by the Stober process171 demonstrate that nucleation and growth occur by a coagulative mechanism, which supports the description of the gel structure given above. The analysis of the diffraction curves in the Porod region leads to the computation of the fractal dimension (df). The quantity is dependent on the shape and geometry of the diffraction centers and also indicates a possible growth mechanism. Table I11 reports156 the value of the fractal dimension of the sols near the gelation point. These values suggest a percolation cluster (PC) or a diffusion-limited aggregation (DLA) mechanism. Particles grow by addition of small polymeric units to randomly added sites on a nucleus (PC) or through a random walk to a seed cluster (DLA).152 This description is in good agreement with the observation of a structure composed of agglomeration of units of different sizes: secondary particles made of several primary particles, which in turn agglomerate to form a gel. In conclusion, the Keefer fractal model yields a range of fractal dimensions from 1.6 to 2.4 depending on the degree of hydrolysis. As the fractal dimension increases, the pore radius of the resulting gel should decrease. This relates well with the work of Orcel and others, where the degree of hydrolysis and condensation (or reaction rates) determine the pore-size distribution. The effects of adducts such as OH, HF, ammonia, or formamide control the rate of hydrolysis by raising the activation energy for the removal of water in order for condensation to occur. V. Theoretical Studies A. Hydrolysis and Condensation Two models for the Si(OR)4 hydrolysis reaction have been proposed, one in which a trivalent'72 and another in which a penta~alentl~~ transition state is formed. Zerda and Hoang's using high-pressure Raman spectroscopy to study the hydrolysis of TMOS indicates that the model involving a pentavalent transition is correct. In the case of base catalysis, eq 33, the reaction OH- + GSCOCH, - GSi-OCli3- + ZSi-OH + OCHY (33) AH is caused by a hydroxyl ion. The OH- ion has high nucleophilic power and is able to attack the silicon atom directly. These attacks are aimed toward the silicon atom since the Si atom carries the highest positive Hench and West charge. At acidic conditions, the proton is attracted by the oxygen atom of the OCH, group, eq 34. This causes H I _ H30+ + esi6ch3 + E S i H 3 - I HZO ESi4I-l + CH30H + H+ (34) a shift of the electron cloud of the Si-0 bond toward oxygen, and as a result the positive charge of the silicon atom increases. A water molecule can now attack the silicon atom, and a transition state is formed.174 The hydrolysis reaction is sufficiently slow that its dynamics can be studied by using high-pressure Raman spectroscopy, as shown by Zerda and H0a11g.l~~ For the first-order kinetics, the reaction rate constant is found from the slope of the logarithmic plot of the concentration of the reactant against time. Because the magnitude of Raman bands is proportional to the concentration of the molecules in the system, the reaction rate can be found from the time dependence of the band intensity. The pressure dependence of the reaction rate is related to the volume of a~tivation.l~~j~~ At a ph varying from 4.9 to 7.5 and at a 1:lO molar ratio of TMOS to water, Zerda and Hoang determined the volume of activation, AVO, and its intrinsic, AVi, and solvent, AV,, components. AVi represents the change in the volume due to changes in bond lengths and angles. It is negative when a new bond is formed. AV, represents the change in volume due to changes in surrounding medium (electrostriction) during the activation step. Analysis of the results174 (AVO = -52 f 10, AVi = -2, AV, = -50 cm3/mol) showed that in the transition state the silicon atom is in a pentavalent state. This was the first experimental proof for the pentavalent state of silicon in the transition stage of the hydrolysis reaction. These experimental results confirm a series of theoretical calculations. Davis and B~rggrafl~~-" have proposed mechanisms, based upon quantum mechanical calculations, for anionic silanol polymerization in which participation of hypervalent siliconates is important. As noted above hypervalent silicon is an important candidate as an intermediate in this chemistry. Strong anionic nucleophiles have been shown to form pentacoordinate complexes with silanes without activation in the gas phase.181 Also, certain pentacoordinate siliconates are readily stabilized in solution.182 An important key to understanding silanol polymerization chemistry is identifying how water is eliminated as the polymerization proceeds. Davis and Burggraf s calculation^'^^-^^ suggest that water is more readily eliminated from hypervalent siliconates than tetravalent silicates in hydroxide-catalyzed silanol polymerization. However, accurate prediction of the entire process of water elimination using an MNDO program is difficult because MNDO overpredicts dissociative activation energies and does not model hydrogen bonding interactions.182 These faults are due to overestimation of core-core repulsions between atoms when they are separated by approximately van der Waals distances. The AM1 semiempirical program has largely overcome this drawback; see refs for details. Consequently, Burggraf and Davida2 have modeled silicic acid reactions using AM1 to predict siliconate elimination reactions as influenced by other nucleo-
15 The Sol-Gel Process Chemical Reviews, 1990, Vol. 90, No philic species that can complex to form hypervalent intermediates. They applied semiempirical molecular orbital calculations to examine the formation of pentacoordinate silicic acid complexes with hydroxide ion and fluoride ion, as well as neutral adducts with hydrogen fluoride, ammonia, and formamide. They also have calculated reaction paths for water elimination from silicic acid complexes with hydroxide ion, fluoride ion, and hydrogen fluoride. The qualitative semiempirical picture of the reaction surface has been quantified by employing high-level ab initio calculations for selected intermediates and transition-state structures. The adducts studied were chosen because of their potential as catalysts or drying control agents in sol-gel processing chemistry. For example, as discussed earlier, formamide is used as a drying control additive for sol-gel chemistry to control the ratio of rates of siloxane hydrolysis and silanol polymerization. The semiempirical methods used in Davis and Burggrafs research are part of the MOPAC program available from the Quantum Chemistry Program Exchange (QCPE) at the University of Indiana.lE3 Semiempirical molecular orbital calculations were performed using MNDO6 and AM17 methods developed by Dewar and c~-workers.'~j~~ Revised silicon parameters were used for MNDO All stationary points on the potential surfaces were fully optimized by using procedures of the MOPAC program. Force constant calculations and intrinsic reaction coordinate calculations were performed for each stationary point to determine the nature and connectivity of the potential surface. Ab initio calculations were performed using the GAUSSIAN86 program and basis sets it contains.'s7 All ab initio calculations in their work were single-point calculations at AM1 geometries. Estimates of energies at the MP1/6-31++G(d) were calculated by assuming correlation effects and polarization effects are Comparisons of ab initio results and semiempirical results are used to establish a quantitative benchmark for semiempirical energies in order to solve problems that are too large for high-level ab initio methods.lg2 For reaction of any nucleophile with silicic acid, two possible outcomes are (1) addition and (2) abstraction. By studying the possible reaction paths for the removal of water, the proton-abstracting pentacoordinated silicon has no activation energy for water removal. In contrast, the pentavalent silicon has a relatively large activation energy for removal of water if the proton is added and constrained to form its most stable structure before the water is removed. Figure 17 shows both the proton abstraction and hydroxyl paths that include the addition of pentacoordinated silicon as an intermediate in the condensation reaction. The more favorable proton abstraction path is one where a proton from a silanol moves toward the hydrogen-bonded OH as the OH moves toward the silicon. This forms a pentacoordinated silicon intermediate where water easily escapes. If, on the other hand, the OH is moved toward the silicon to form a stable pentacoordinated structure, the energy is much lower. From this structure, a significant activation energy is then required to eliminate the water. 1.. ta Forrr Watw: 51 (OH 'Kp -50 DrotonA Addition = -93 +,( -103 SI(OH)~ f Condensation, React ion Coordinat ion Figure 17. Formation of pentacoordinate silicon. Burggraf and Davisla2 used MNDO, AM1, and ab initio molecular orbital models to predict the proton abstraction and resulting pentacoordinate silicon. They constructed similar models for HF ammonia and formamide adducts on silicic acid. For HF they also predict that the pentacoordinated silicon created by proton abstraction is the more favorable path to water elimination. The difference is that water elimination from HF adducts has a slight energy barrier. This indicates a shift to a slower condensation rate for the HF-silanol system over the OH-silanol system. Ammonia and formamide adducts with silicic acid form by hydrogen bonding. Formamide is predicted to form a bistable bond in which one oxygen-silicon bond is shorter than the other. The long bond oxygens permit more favorable hydrogen-bonding interactions. Burggraf and DavislE2 also calculated the energy of water adducts on silicic acid. They found that there were very small energy differences between the pentacoordinated water adducts and the corresponding hydrogen-bonded water adducts. This result is important when considering the effect of water adducts on rings of silica tetrahedra discussed in a later section. B. Gelation In the previous sections, we saw that experimental analyses of silica gelation using SAXS, Raman spectroscopy, and a Mo dissolution technique led to the conclusion that a gel network is preceded by the formation of very small clusters, or primary particles, of silica tetrahedra. The primary particles are apparently formed by polycondensation that favors nearly closed clusters of tetrahedra rather than linear chains. This conclusion regarding the gelation and resulting ultrastructure of acid-catalyzed alkoxide-derived silica gels has been tested by West et al.lg3 and Davis and Burggraflg4 using semiempirical quantum calculations. The calculations done by West et al. used an intermediate neglect of differential overlap (INDO) molecular orbital mode1.1g3 The INDO program was made available by the Quantum Theory Project at the University of F10rida.l~~ The calculations done by Davis and Burggraf used the AM1 mode1.1g4 The silica structures evaluated contain from one to six silica tetrahedra. In each model two bridging oxygens and two nonbridging oxygens are bonded to each silicon. One hydrogen is bonded to each of the nonbridging oxygens to terminate the structure and balance the charge. Both ring and chain models of silica tetrahedra were evaluated, and their energies compared.
16 48 Chemical Reviews, 1990, Vol. 90, No Uncorreclee for water Secondav I particle Hench and West Figure 18. Q 4 TABLE VI. INDO Calculations for Silica Structures INDO no. of silica energy per HOMO-LUMO uv cutoff tetrahedra struct Tetrahedra, au wavelength, nm 1 tetrahedra chain ring chain ring chain ring chain ring chain ring rr JJ , Figure 18 shows the 2-D projections of chain and ring structures for four silica tetrahedra that have been geometrically optimized to minimize the molecular energy by using INDO calculations. These projections are typical of the hydroxylated silica structures modelled by West et al.lg3 and Davis and Burggraf.lg4 The clusters were each optimized for the minimum energy by using a molecular mechanics (MM2)'% routine. The molecular orbitals were determined by using geometrically optimized INDO calculations. The molecular energies were evaluated and compared to establish the relative stability of each structure. The energy gap between the highest occupied molecular orbital (HOMO) and the lowest unoccupied molecular orbital (LUMO) for the single states and the corresponding UV cutoff wavelength were determined. The calculated optical properties are compared with experimental values in the properties section of this review. Table VI, summarizing the INDO calculations, is shown to compare the relative stability of the INDO structures. The more negative the energy, the more stable the structure. These differences are exaggerated because each chain structure has an extra water mole- Figure Number of SI tetrahedra TABLE VII. Cluster Sizes for Rings and Chains of Tetrahedra no. of silica cluster size, A INDO tetrahedra N rings chains (chain-ring), au cule when compared to the ring structure. Figure 19 shows the INDO energy per silica tetrahedra for rings and chains as a function of the number of tetrahedra. It suggests that the chain structures are more stable than the rings for small number of silica tetrahedra. This has been observed experimentally by Klemperer and Ramamurthig7 and Orcel and Hench1lG using NMR spectroscopy, where a linear, as opposed to a ring, growth model most consistently interprets the experimental structural evidence prior to gelation. As mentioned earlier, investigatorsg4 have proposed models for the structure of acid-catalyzed silica gels containing two levels of structure formed before gelation. These models propose the formation of primary particles, of diameter 1-2 nm, which agglomerate to form secondary particles of about 4-6 nm before drying. The secondary particles give rise to the pore structure after drying. Table VI1 shows the differences in the INDO structural energies between chains and rings (C-R). The relative stability of chains compared to rings decreases as the number of silica tetrahedra increases by the decrease in the difference between their calculated INDO energies. The difference is estimated to reach zero as the number of tetrahedra reaches about 10 or 12, when the driving force for rings becomes more favorable than for chains. This result is similar to the size range where secondary particle growth stops in acidic silica Acid catalysis ensures complete hydrolysis of the silica tetrahedra, as used in these calculations. The size of the INDO-calculated rings or clusters for tetrahedra appears to fall within the range of the radius of gyration of the primary particles calculated from SAXS analysis of acid-catalyzed silica so1s.94j56 As gelation occurs, the cross-linking of the structure becomes more dominant. A statistical analysis conducted by Zarzyckis1 indicates that chain growth is limited by this process and rings must be formed. The energy differences in the ring structures in the INDO model are very small. This indicates that a broad distribution of ring sizes may be possible in a gel as they
17 The Sol-Gel Process Chemical Reviews, 1990, Vol. 90, No " Number of Si tetrahedra Figure 20. AMI corrected energy difference. TABLE VIII. AM1 Enthalpies of Rings and Chains at 25 "C (kcal/mol) no. of silica AHf tetrahedra N chain ring water differences become energetically more favorable. Davidg4 recalculated the energetics of rings and chains using AM1. His calculations were corrected for the extra water molecule in the chains as compared to the rings. The AM1 energies were also corrected for zero-point energy and converted to enthalpies at 25 "C. These corrections moved the crossover energy from 10 to 12 tetrahedra to 3 or 4 tetrahedra (see Figure 20). Table VI11 shows the enthalpies, AH,, in kcal/mol for rings and chains and their differences. Chains are still the most likely to occur in the early stages of hydrolysis and condensation. The important feature is that chains and rings are reversed in energy difference when three to four tetrahedra or more are formed. The driving force to produce chains is eliminated, and therefore 4-fold rings are very likely. This corresponds very closely to the 1-2-nm primary silica particles that form prior to agglomeration, as shown in Tables I11 and VII. Thus, results from quantum mechanical calculations compare quite favorably to experimental observations for the ultrastructure development in alkoxide-derived sili~as.'~~-~~~ VI. Aghg When a gel is maintained in its pore liquid, its structure and properties continue to change long after the gel point. This process is called aging. Four processes can occur, singly or simultaneously, during aging, including polycondensation, synerisis, coarsening, and phase transformation. Although there is an extensive literature on aging by Iler,15*76J20 and Scherer has made an effort to describe aging phenomena theoretically,7 *205 there is relatively little detailed knowledge of aging mechanisms and kinetics and even less quantitative analysis of the effects of aging on gel structure and properties.206 Polycondensation reactions, eqs 3 and 4, continue to occur within the gel network as long as neighboring silanols are close enough to react. This increases the connectivity of the network and its fractal dimension. Syneresis is the spontaneous shrinkage of the gel and resulting expulsion of liquid from the pores. Coarsening is the irreversible decrease in surface area through dissolution and reprecipitation processes. Disintegrated op Figure 21. Stages in aging of gel: (A) Gel as formed and dried. Shrinks on drying, giving small pore volume and pore diameter. (B) Wet heat-aged-increased coalescence. Little shrinkage on drying. Pore diameter larger than the dried sample A. (C) Further heat aged or autoclaved. Structure-coarsened small area and large pores but same pore volume as sample B. (D) Disintegration to irregular round particles. A. Polycondensation Usually in alkoxide-based gels the chemical hydrolysis reaction is very rapid and is completed in the early stage of sol preparation, especially when the sol is acid catalyzed. For silica gels synthesized in alcoholic solutions, i.e., made by hydrolysis and condensation of alkoxides, nuclear magnetic resonance (NMR,207p208 Figure 21) and Raman spectroscopies209 show that the number of bridging bonds increases long after gelation. The condensation reaction continues to occur because of the large concentration of silanol (SiOH) groups in a newly formed gel. As the hydroxyls are lost during aging, new bonds are formed, creating more cross-linked structures. 29Si NMR results of Kelts et al.'07 show substantial amounts of Q2 species at the gel point, and the proportions of Q3 and Q4 species increase with time long after gelation. As discussed earlier, &" represents a Si atom bonded through a bridging oxygen to n other Si atoms. Since the chemical reaction is faster at higher temperature, aging can be accelerated by hydrothermal treatment, which increases the rate of the condensation reaction. B. Syneresis The shrinkage of the gel and the resulting expulsion of liquid from the pores is called syneresis.76~205*210 Syneresis in alcoholic gel systems is generally attributed to formation of new bonds through condensation reactions, which increases the bridging bonds and causes contraction of the gel network. In aqueous gel systems, or colloidal gels, the structure is controlled by the balance between electrostatic repulsion and attractive van der Waals forces. Therefore, the extent of shrinkage is controlled by additions of electrolyte. Vysotskii and colleagues211*212 have shown that the rate of contraction of silica gel during syneresis has a minimum at the isoelectric point (IEP). For silica this point is at a ph of 2, at which the silicate species are un-
18 50 Chemical Reviews, 1990, Vol. 90, No. 1 Hench and West charged.76 Since the condensation is the slowest at that point, this suggests that the shrinkage is driven by the condensation reaction in eq 3. It has also been suggested by that contraction is driven by the tendency to reduce the huge solid-liquid interfacial area of the gel. This might be accomplished by flexure of the solid phase, bringing surfaces into contact, in which case it would be indistinguishable from the reaction-driven mechanism. That means the chemical potential of the gel is reduced by both chemical reactions (since the condensation reaction is exothermic) and the reduction in the solid-liquid interfacial area. But Scherer also shows that the latter suggestion is not supported by experimental results.83 The syneresis contraction rate increases with concentration of silica in the sol and with temperature. When organic solvents are present, they may form hydrogen bonds with the silanol groups, which inhibit condensation and slow syneresis. Vysotskii and Strazhesko show that the rate of syneresis decreases with time.z11 This could result from the increasing stiffness of the network as more bridging bonds are formed. Ponomareva et al.213 found that the total syneresis strain is greater at lower temperatures, although the contraction rate is slower. They argued that at higher temperature the condensation reaction is faster, so the gel becomes stiff faster and shrinkage is prevented. If this is so, it implies that the shrinkage is not proportional to the scale of reaction. They conclude each bond does not cause a certain amount of strain. Another factor that may affect the rate of contraction is the permeability of the gel to the flow of liquid in the pores. C. Coarsening Another process, called coarsening or Ostwald ripening, is discussed at length by and co-worke r ~ Since. ~ ~ convex ~ surfaces are more soluble than concave surfaces, if a gel is immersed in a liquid in which it is soluble, dissolved material will tend to precipitate into regions of negative curvature. That means that necks between particles will grow and small pores may be filled in, resulting in an increase in the average pore size of the gel and decrease in the specific surface area. Since the solubility of silica increases at high ph, so does the rate of coarsening of silicate gels. It is not surprising that the rate of coarsening of gels is similarly ph dependent. The pore-size distribution in a silica xerogel increases as a result of aging in a basic solution. At a given normality, Sheinfain et al.z15 found the effect of solution on aging to decrease in the order HC1 > H2S04 > H,PO,; however, the rate of aging was independent of the type of acid if the activity of the proton was the same in each solution. They examined the coarsening of silica gels in concentrated mineral acid (1 < ph < 2) and showed that silica is even soluble at very low ph. Iler76 provides a number of references concerning the change in the surface area and the pore size during aging. The reduction in surface area is produced by dissolution and reprecipitation. A high pore volume results because the stiffer gel produced by aging does not shrink as much under the influence of capillary pressure. Okker~e ~ has shown that the texture of silica can be affected in every stage of its preparation, including gelation, after-treatment of the hydrogel by aging and washing with various liquids, and drying. These influences can be qualitatively understood and predicted on the basis of a condensation theory of aging. This theory attributes a major role to the rate of the condensation reaction of silicic acid in all stages during the development of the texture. D. Processlng Parameters That Affect Aging Time, temperature, and ph are parameters tht can effectively alter the aging process. Ilerlz2 recognized that once the gel structure has been formed it can be further modified in the wet state by treatment to (1) strengthen the structure without greatly affecting the pore structure (sometimes referred to a gel reinforcement) or (2) enlarge the pore size and reduce the surface area by a process of dissolution and redeposition of silica, thereby coarsening the gel texture. Sheinfain et al2l5 recognized the first two distinct stages in the thermal-aging process. The more extensive the wet aging, the subsequently dried gel shrinks less and the pore volume and diameter are greater, but there is very little change in surface area. Second, upon further aging the surface area begins to decrease while the pore size continues to increase. However, there is then little further change in pore volume. The explanation is clear from the stages of aging shown in Figure 21. The first stage involves only an increased coalescence or bonding between the ultimate particles which strengthens the gel so that it shrinks less upon drying. Heating the gel in water until the specific surface area has been reduced by 1040% can strengthen the weak gel structure. Heating gel in water at C generally brings about reinforcement but does not modify the pore structure. It is interesting that at 80 C Liu showedzo6 there was no effect unless the gel had a surface area greater than 200 mz/g. Prolonged aging of silica gel with an initial surface area of 920 mz/g in water at ph 6.8 at room temperature was carried out by Sheinfain et al.z15 The surface area dropped from 725 to 420 m2/g, while the pore radius increased from 9 to 43 A. However, the porosity also increased from 0.31 to 0.90 cm3/g. The structure was thus strengthened so that shrinkage upon drying was reduced. The reinforcement was striking when samples were first washed with acetic acid and then dried. Since the surface tension of acetic acid is only one-third that of water, the reinforced gel had a much higher pore volume of 2.36 cm3/g, which is a low-density gel. The rate of coarsening of silica increases with temperature and pressure, as discussed by Iler.76 Aging in water above 100 C under pressure in an autoclave brings about far greater structural changes than can be obtained at 100 C. Van der Grift et a1.216 prepared silica gels by neutralization of alkaline silicate solutions and aged them in an autoclave in water at various temperatures. When the temperature was above the boiling point of water, the sample was exposed to steam at high pressure, resulting in hydrothermal aging. Washing the pore liquor out of a gel is also an aging step, and the ph of the wash water is critical in the case of gels made from acid-catalyzed silicate precursors. The final properties of such gels depend on both the ph at which the gel was formed and the ph in which
19 The Sol-Gel Process it was washed (aged) before drying. For example, Okkerse et al.217 heated a series of gels for 1-4 days at 80 "C in water, acid, and potassium chloride solutions and found that if the gel had a specific surface area greater than about 200 m2/g, then it underwent a decrease in surface area. There was little effect at ph 2, but in neutral or alkaline solution, especially in the presence of salt, the gel texture was markedly coarsened. For example, the surface area decreased from 752 to 452 m2/g while pore radius increased from 13 to 22 A, but volume remained at 0.5 cm3/g. Soaking a silica gel in dilute ammonium hydroxide solution at "C can result in drastic coarsening of the gel texture. Girgis218 reported that even soaking a silica gel at ph for 1 day at 20 "C caused the surface area to drop from 650 to 467 m2/g with a corresponding increase in pore radius. It might be thought that since silica does not dissolve at low ph, acids would have little effect on wet aging other than to adjust ph. However, Sheinfain et al.215 found that treating the gel with strong acids, HC1, HNO,, or concentrated H2S04 before drying increases the pore volume of the dried gel without lowering the surface area. This is because the acid promotes coalescence between particles without particle growth and coarsening of the texture. On the other hand, 8 N HzSO4 caused a drop in surface area from 700 to 300 m2/g and at the same time increased the pore volume.215 Thus, strong acids (ph < 2) promote the aging of silica gel but, unlike alkalis as an aging promoter, cannot dissolve the gel if added in excess. It is seen that aging and thermal treatments result in a one-way process: loss of specific surface area and an increase in pore size. The pore size can be enlarged also by dissolution of some of the silica. Sheinfain et al.215 reported that treating a gel with 0.5 N KOH or dilute HF can enlarge the pores from 0.7 to 3.7 nm. If silica were dissolved away evenly from all the surface, there should be an increase in specific surface. However, it is probable that regions of lower radius of curvature will dissolve more rapidly so that the specific area may actually decrease. The fractal nature of a gel will also be a major influence on the gelation and aging process as discussed earlier.219 Condensation reactions between gel network segments will be more important when the number of interconnections is large.151 E. Properties During aging, there are changes in most physical properties of the gel. In the study of aging kinetics of silica gel, the textural properties &e., pore size, porosity, and surface area) are of great importance. With respect to drying behavior, it is the change in mechanical properties during aging that is most important. Inorganic gels are viscoelastic materials responding to a load with an instantaneous elastic strain and a continuous viscous deformation. Since the condensation reaction creates additional bridging bonds, the stiffness of the gel network increases, as does the elastic modulus, the viscosity, and the modulus of rupture. This is illustrated in Figure 22, which shows the increase in modulus of rupture of silica gel during aging for a gel with a water/tmos ratio of 16/1.220 The modulus of rupture of a gel aged at 105 "C reaches 40 Pa by 40 - A n v) a w K a I- n. 3 a Chemical Reviews, 1990, Vol. 90, No RUPTURE MODULUS ABOVE 90 C Q I.,., DAYS Figure 22. Rupture of modulus of wet gel (made from TMOS) versus aging time.220 days. West et al.220 showed that gel strength increased logarithmically with times ranging between 1 and 32 days. The strength increased exponentially with temperature between 25 and 105 "C. The strongest gels produced had rupture moduli of approximately 400 Pa. Similar data were obtained by Pardenek et a1.221 for polymer gels as well as for colloidal gels made from fused silica. Dumas et followed the shear modulus for 9 months in gels made from TEOS and found that it continued to increase. The strength of the gel also increased with aging. For that reason, it is advisable to age large monolithic gels before drying to reduce the chance of ~racking.~~.~~ The greater stiffness of the aged gel reduces the shrinkage during drying as mentioned before, especially if the aging treatment is performed under hydrothermal conditions. VII. Drying The drying behavior of porous solids has been extensively studied by Sher~ood,~~~-~~~ Keey,226 Mujumdar,227i228 Moore,2m Whitaker,230 Cooper,231 Ford,232 and S~herer.~~,~~-~y~~~ However, most of the data have been on powder systems with relatively large pores. Even the few quantitative studies conducted on gels by Kawaguchi et al.234 and D~ivedi~,~ have been on large pore gels. Consequently, theoretical analyses of gel drying such as by or by Zarzyckis1 using Cooper's model for ceramic powders231 have been based upon classical concepts of drying. It has been generally accepted since the time of Sher~ood~~*~~~-~~~ that there are three stages of drying: Stage 1: During the first stage of drying the decrease in volume of the gel is equal to the volume of liquid lost by evaporation. The compliant gel network is deformed 2
20 52 Chemical Reviews, 1990, Vol. 90, No. 1 Hench and West by the large capillary forces, which causes shrinkage of the object. In classical large-pore systems, this first stage of drying is called the constant rate period because the evaporation rate per unit area of the drying surface is independent of A detailed review of the drying phenomena associated with the constant rate period is presented in Brinker and S~herer.~~ This behavior is applicable to gels made by colloidal precipitation (method 1) or base-catalyzed alkoxide gels (method 3) that have pores >20-nm average diameter. However, a recent quantitative analysis by Wilson237 and Wilson and H e n ~ h of ~ the ~ ~ drying q ~ ~ kinetics ~ of acid-catalyzed alkoxide gels shows that for gels with pores <20 nm the rate of drying in stage 1 is not constant but in fact decreases substantially. As discussed below, this behavior is due to changes in pore radii during drying, which cause substantial reductions in vapor pressure of the liquid in the small pores. For large or small pore gels the greatest changes in volume, weight, density, and structure occur during stage 1 drying. Stage 1 ends when shrinkage ceases. Stage 1 ends and stage 2 begins when the critical point is reached; classical drying theory calls this the leatherhard point The critical point occurs when the strength of the network has increased, due to the greater packing density of the solid phase, sufficient to resist further shrinkage. As the network resistance increases, the radius of the meniscus is reduced. Eventually, at the critical point, the contact angle approaches zero and the radius of the meniscus equals the radius of the pore. This condition creates the highest capillary pressure, and unable to compress the gel any further, the pores begin to empty, which is the start of stage 2. In stage 2 liquid transport occurs by flow through the surface films that cover partially empty pores. The liquid flows to the surface where evaporation takes place. The flow is driven by the gradient in capillary stress, as described by Whitaker.241 Because the rate of evaporation decreases in stage 2, classically this is termed the first falling rate period Stage 3: The third stage of drying is reached when the pores have substantially emptied and surface films along the pores cannot be sustained. The remaining liquid can escape only by evaporation from within the pores and diffusion of vapor to the surface. During this stage, called the second falling rate period,225 there are no further dimensional changes but just a slow progressive loss of weight until equilibrium is reached, determined by the ambient temperature and partial pressure of water. Whitaker has developed a theoretical analysis of the second falling rate period. Brinker and Scherer70 review the factors in this stage that are relevant to the drying of gels. A comparison of Dwivedi s results235 on the drying of an alumina gel with those of Wilson and H e n ~ h ~ ~ ~ * ~ ~ ~ for an acid-catalyzed alkoxide silica gel illustrates the importance of pore size in gel drying behavior. Dwivedi prepared the alumina gels using the Y01das~~ method, which yields gels with pores >>20 nm. Samples up to 3 mm thick were weighed at periodic intervals during drying at 80 C. Figure 23, from D~ivedi,2~~ shows that the rate of water loss was constant from his gels during stage 1 (within the range of the considerable experimental error caused by removing the sample from the oven for weighing). He showed that the rate was similar.- c E 0.20 N 6 0) 0.15 v u) u) First Stage Second Stage L 4 P (L, u m , m CI: - Evaporation rate of T distiled water - - L ILL I I